10-1.__ RUBBERIZED BONDED WEARING COURSE - OPEN GRADED
This work includes producing and placing bonded wearing course. Bonded wearing course
consists of rubberized hot mix asphalt (open graded) (RHMA-O) placed over a membrane of
polymer modified asphaltic emulsion in a single pass with an integrated paving machine.
Comply with the specifications for RHMA-O under Section 39, "Hot Mix Asphalt," of the
Standard Specifications. Use the Standard construction process.
With the job mix formula (JMF) submittal, submit target residual rate for asphaltic emulsion
Within 3 business days following the first delivery, submit test results for asphaltic emulsion
properties performed on a sample taken from the asphaltic emulsion delivered. Test results must
be from an AASHTO accredited laboratory. Test results must comply with the table "Asphaltic
Within 1 business day of each job site delivery of asphaltic emulsion, submit to the
Transportation Laboratory a 2-quart sample and a Certificate of Compliance in compliance with
Section 6-1.07, "Certificates of Compliance," of the Standard Specifications. Ship each sample
so that it is received at the Transportation Laboratory within 48 hours of sampling. Label each
asphaltic emulsion sampling container with:
1. Emulsion producer and location
2. Asphaltic emulsion type
3. Percent of water
4. Application rate
5. Sampling location and date
6. Contract number
Each day bonded wearing course is placed, submit the residual rate and the application rate
for asphaltic emulsion membrane.
During production, submit certified volume or weight slips for the materials supplied.
Quality Control and Assurance
Do not test RHMA-O aggregate for tensile strength ratio.
Sample RHMA-O from either a truck or the material transfer device (MTV) hopper.
Perform sampling and testing at the specified frequency for the following additional quality
Minimum Quality Control
Quality Test and Testing Sampling
Characteristic Method Frequency Specification Location
Various At least Specified in "Materials" Delivery truck
ASTM once per Submitted target application rate ± 0.02 QC Plan
D 2995 paving day gallons per square yard At the job site
The Engineer samples and tests for the following additional quality characteristic for
Quality Characteristic Test Method Specification Sampling Location
Various Specified in "Materials" Delivery truck
Submitted target residual rate ±
membrane ASTM D 2995 At the job site
0.02 gallons per square yard
Sample asphaltic emulsion under AASHTO T 40. For each job site delivery of asphaltic
emulsion, take a 2-quart sample in the presence of the Engineer. Take samples from the delivery
truck mid-load from a sampling tap or thief. If the sample is taken from the tap, draw and
discard 4 quarts before sampling.
If you unload asphalt binder or asphaltic emulsion into bulk storage tanks, do not use
material from the tanks until you submit test results for a sample taken from the bulk storage
tank performed by an AASHTO-accredited laboratory.
Asphaltic Emulsion Membrane
Asphaltic emulsion membrane must comply with:
Asphaltic Emulsion Membrane
Properties Test Method Min. Max.
Saybolt-Furol viscosity, at 25 C, s AASHTO T59 20 100
Sieve test on original emulsion (at time - 0.05
of delivery), %
24-hour storage stability (see note), % - 1
Residue by evaporation, % California 63 -
Tests on residue from evaporation test:
Torsional recovery, measure entire arc of California 40 -
recovery, at 25 C, % Test 332
Penetration (0.01 mm) at 25 C AASHTO T49 70 150
Note: After standing undisturbed for 24 hours, the surface must be a smooth
homogeneous color throughout and show no white, milky colored substance.
Asphalt binder mixed with asphalt modifier and crumb rubber modifier (CRM) for asphalt
rubber binder must be PG __.
Aggregate for RHMA-O must comply with the ___ OGFC grading.
Before the addition of asphalt binder and lime treatment, aggregate must comply with:
Quality Characteristic Test Method Requirement
Percent of crushed particles CT 205
Coarse aggregate (% min.)
Two fractured faces 90
Fine aggregate (% min)
(Passing No. 4 sieve and retained on No. 8 sieve.)
One fractured face 85
Los Angeles Rattler (%, max.) CT 211
Loss at 100 Rev. 12
Loss at 500 Rev. 35
Sand equivalent a (min.) CT 217 47
Fine aggregate angularity (%, min.) AASHTO 45
T 304 Method A
Flat and elongated particles ASTM D 4791
(% max. by weight @ 3:1) 25
Reported value must be the average of 3 tests from a single sample.
Reclaimed Asphalt Pavement
Do not use reclaimed asphalt pavement in bonded wearing course.
HOT MIX ASPHALT DESIGN REQUIREMENTS
Asphalt Rubber Binder Content
The Engineer uses the following formula to determine the optimum asphalt binder content
OBC2 = (OBC1) x 1.40
OBC1 = Optimum bitumen content using the specified PG
asphalt binder under California Test 368.
OBC2 = Optimum bitumen content using asphalt rubber
Treat aggregate with the same antistrip treatment used for HMA Type ___.
Attendance at the prepaving conference is mandatory for:
1. Emulsion supplier
2. Paving foreman
3. RHMA-O supplier
4. Project superintendent
5. Project Manager
Do not store RHMA-O more than 4 hours.
Spreading and Compacting Equipment
Use an integrated distributor-paver capable of spraying the asphaltic emulsion membrane,
spreading the RHMA-O, and leveling the mat surface in 1 pass.
Apply asphaltic emulsion membrane at a uniform rate for the full paving width. The
asphaltic emulsion membrane must not be touched by any part of the paver including wheels or
If the spray bar is adjusted for changing pavement widths, the paver must prevent excess
spraying of asphaltic emulsion beyond 2 inches of the HMA edge.
Use a material transfer vehicle (MTV) to receive RHMA-O directly from the truck and
deliver to the paver's receiving hopper or feed system. The MTV must:
1. Remix the RHMA-O with augers before loading the paver
2. Have sufficient capacity to prevent stopping the paver
The paver must have a full-width, heated vibratory screed that uniformly spreads and finishes
Compact RHMA-O with steel-tired, 2-axle tandem rollers. Each roller must weigh from 126
to 172 pounds per linear inch of drum width.
Transporting, Spreading, and Compacting
Apply asphaltic emulsion membrane on dry or damp pavement with no free water. Apply
asphaltic emulsion when the atmospheric and pavement temperatures are above 50 °F.
Before spreading RHMA-O, apply asphaltic emulsion membrane under Section 94,
"Asphaltic Emulsions," of the Standard Specifications. Apply emulsion at a temperature from
120 to 180 F and in a single application at the residual rate specified for the condition of the
underlying surface. Choose a target residual rate from the following:
Asphaltic Emulsion Membrane Target Residual Rate
Surface to Receive Asphaltic Emulsion Membrane Target Residual Rates (gallons per square yard)
PCC pavement 0.09 - 0.11
Dense, compacted, new HMA pavement 0.11 - 0.14
Open textured, dry, aged or oxidized AC pavement 0.13 - 0.17
If you request and the Engineer approves, you may change asphaltic emulsion membrane
Construct a transverse joint when RHMA-O remains in the paver for more than 30 minutes.
Spread RHMA-O after applying asphaltic emulsion membrane and before the asphaltic
emulsion membrane has spread beyond the area to be covered by the RHMA-O. Do not apply
asphaltic emulsion membrane more than once
Do not reintroduce into the paving process RHMA-O spread over asphaltic emulsion
Do not overlap or hot lap RHMA-O. Pave through lanes after paving adjacent:
4. Road connections
6. Curve widenings
7. Chain control lanes
9. Turn pockets
For bonded wearing course placed on areas adjacent to through lanes that extend into the
through lanes, cut the bonded wearing course to a neat vertical line at the lane line.
If you spill asphaltic emulsion into the paver hopper, stop paving and remove and dispose of
the contaminated material.
When measured on the surface immediately behind the screed, the RHMA-O must be at least
280 F and the temperature across the mat should not vary by more than 25 F. Do not take the
temperature within 2 feet of the edge of the pavement.For each paver used, compact RHMA-O
with 2 coverages using 2 rollers with the vibrators turned off. Complete the first coverage before
the surface temperature drops below 270 °F. Complete all compaction before the surface
temperature drops below 250 °F.
If the atmospheric temperature is below 70 °F, cover loads in trucks with tarpaulins. The
tarpaulins must completely cover the exposed load until you transfer the mixture to the MTV.
You may omit tarpaulins if the time from discharge to truck until transfer to the MTV is less than
Do not allow traffic on bonded wearing course until the surface temperature is below 160 °F.
If bonded wearing course is placed over HMA constructed under the same project:
1. The top layer of the HMA must comply with smoothness specifications before placing
bonded wearing course.
2. Bonded wearing course must comply with straightedge and must-grind specifications.
For bonded wearing course placed over existing asphalt concrete, only the straightedge
specifications for smoothness apply.
Remove and replace bonded wearing course not complying with the must-grind and
straightedge specifications, except you may grind bonded wearing course for correcting
1. At a transverse joint separating the bonded wearing course from pavement not
constructed under the same project
2. Within 12 feet of a transverse joint separating the pavement from a bridge deck or
Construct rumble strip by grinding indentations.
If you perform half-width paving, at the end of each day's work the distance between the
ends of adjacent surfaced lanes must not be greater than can be completed in the following day
of normal paving.
Do not leave a vertical joint more than 0.15 foot high between adjacent lanes open to public
Place bonded wearing course on adjacent traveled way lanes so that at the end of each work
shift, the distance between the ends of bonded wearing course layers on adjacent lanes is
between 5 feet and 10 feet. Place additional bonded wearing course along the transverse edge at
each lane's end and along the exposed longitudinal edges between adjacent lanes. Hand rake and
compact the additional bonded wearing course to form temporary conforms. You may place
Kraft paper or another approved bond breaker under the conform tapers to facilitate the taper
removal when paving operations resume.
Place shoulder conform tapers concurrently with the adjacent lane's paving.
Place additional RHMA-O along the pavement's edge to conform to road connections and
private drives. Hand rake, if necessary, and compact the additional RHMA-O to form a smooth
MEASUREMENT AND PAYMENT
Bonded wearing course is paid for as rubberized hot mix asphalt (Bonded Wearing Course -
Open Graded) and asphaltic emulsion membrane (Bonded Wearing Course). Rubberized hot
mix asphalt (Bonded Wearing Course - Open Graded) is measured and paid for as specified in
Section 39-5, "Measurement and Payment," of the Standard Specifications. Asphaltic emulsion
membrane (Bonded Wearing Course) is measured as specified for asphaltic emulsion in Section
94, "Asphaltic Emulsions," of the Standard Specifications.
The contract price paid per ton for asphaltic emulsion membrane (Bonded Wearing Course)
includes full compensation for furnishing all labor, tools, materials, equipment and incidentals,
and for doing all the work involved in asphaltic emulsion membrane, complete in place, as
shown on the plans, as specified in the Standard Specifications and these special provisions, and
as directed by the Engineer.